Abstract
Strong electron correlations can give rise to extraordinary properties of metals with renormalized Landau quasiparticles. Near a quantum critical point, these quasiparticles can be destroyed and nonFermi liquid behavior ensues. YbRh_{2}Si_{2} is a prototypical correlated metal exhibiting the formation of quasiparticle and Kondo lattice coherence, as well as quasiparticle destruction at a fieldinduced quantum critical point. Here we show how, upon lowering the temperature, Kondo lattice coherence develops at zero field and finally gives way to nonFermi liquid electronic excitations. By measuring the singleparticle excitations through scanning tunneling spectroscopy, we find the Kondo lattice peak displays a nontrivial temperature dependence with a strong increase around 3.3 K. At 0.3 K and with applied magnetic field, the width of this peak is minimized in the quantum critical regime. Our results demonstrate that the lattice Kondo correlations have to be sufficiently developed before quantum criticality can set in.
Introduction
Heavy fermion materials, i.e. intermetallics that contain rare earths (REs) like Ce, Sm, and Yb or actinides like U and Np, are model systems to study strong electronic correlations^{1,2}. The REderived localized 4f states can give rise to local magnetic moments which typically order (often antiferromagnetically) at sufficiently low temperature as a result of the intersite Ruderman–Kittel–Kasuya–Yosida interaction. In addition, the onsite Kondo effect causes a hybridization between the 4f and the conduction electrons, which eventually screens the local moments by developing Kondo spinsinglet manybody states. Hence, these two interactions directly compete with each other and lead to different (longrange magnetically ordered vs. paramagnetic Fermiliquid) ground states^{3}. A zerotemperature transition between the two states can be controlled through doping, pressure or magnetic field H. A quantum critical point (QCP) and concomitantly nonFermi liquid properties ensue if the phase transition is continuous at zero temperature^{4,5,6}.
Heavy fermion metals have been established as a canonical setting for quantum criticality^{2}. How the Kondo lattice coherence develops upon lowering the temperature, i.e. the hierarchy of energy scales, is, however, still a matter of debate. Intuitively, the coherence temperature T_{coh} is set by the singleion Kondo temperature T_{K} of the lowestlying crystalfield level^{7} and can be further reduced by disorder^{8}, while within another model T_{coh} can exceed T_{K} considerably^{9,10}. The latter model might be related to the influence of crystalline electric field (CEF) effects^{2,11}. Considerable experimental efforts have recently been devoted to the study of the quantum critical regime at sufficiently low temperatures. A key observation is that quantum criticality induces a large entropy, suggesting that it is linked with the Kondo effect. This raises the important question^{12} as to how the onset of Kondo lattice coherence at elevated temperatures connects with the emergence of quantum criticality at low temperatures.
The prototypical heavy fermion metal YbRh_{2}Si_{2} shows an antiferromagnetic (AFM) ground state with a very low Néel temperature, T_{N} = 70 mK, and a QCP upon applying a relatively small field μ_{0}H_{N} = 0.66 T parallel to the tetragonal caxis. NonFermi liquid behavior has been observed in the quantum critical regime (i.e. at finite field), extending up to temperatures of about 0.5 K^{13}, depending on the physical quantity that is measured as well as the degree of disorder^{14}, see T–H phase diagram in Fig. 1. Isothermal magnetotransport^{15,16} and thermodynamic^{17} measurements at low temperatures have provided evidence for the existence of an additional lowenergy scale T^{*}(H), which has been interpreted as the finitetemperature manifestation of the critical destruction of the lattice Kondo effect^{18} and the concomitant zerotemperature jump of the Fermi surface from large to small across the QCP. Measurements of the thermal and magnetic Grüneisen ratio strongly support this picture^{19,20}. An ever pressing issue, however, is the huge specific heat coefficient even in zero magnetic field^{14,21}, which implies an abundance of fluctuations. Below T_{N}, these are of Fermiliquid type. Above T_{N}, an obvious cause of these fluctuations are dynamical Kondo correlations, and above ~0.5 K YbRh_{2}Si_{2} at zero field belongs to the quantumcritical fluctuation regime^{13}. Yet, alternative scenarios have been proposed as well^{22,23,24}.
Scanning tunneling spectroscopy (STS) measures locally the density of states (DOS)^{25} through singleparticle excitations^{7,26,27}. Spectra obtained at temperatures T ≥ 4.6 K and H = 0 revealed the successive depopulation of the excited CEF states as the temperature is lowered, with essentially only the lowest crystalfield Kramers doublet occupied at lowest temperatures^{7}. The coupling between the localized 4f electrons in this Kramers doublet and the conduction electrons gives rise to periodic Kondosinglet correlations which start to develop below T_{coh}. This coherence temperature is linked to the effective singleion Kondo temperature T_{K} ≈ 25 K extracted from bulk measurement^{28}. While these properties conform to the traditional understanding of the hightemperature behavior of the Kondo lattice^{29,30}, the questions remain open on how the Kondo coherence evolves further upon lowering the temperature^{13,31,32} and in applied field (green arrows in Fig. 1) and, importantly, how it connects with quantum criticality.
We therefore measure STS down to 0.3 K and in applied magnetic fields up to 12 T, complemented by magnetotransport and thermopower measurements on identical YbRh_{2}Si_{2} samples. We find that lattice Kondo correlations dominate only at temperatures about an order of magnitude below the singleion Kondo temperature. Substantial lattice Kondo correlations are a prerequisite for quantum criticality to set in.
Results
Temperature evolution of tunneling spectra down to 0.3 K
Tunneling conductance curves dI/dV = g(V,T) obtained over a wide range of temperatures are presented in Fig. 2a. Both, the peaks due to CEF splitting of the Yb^{3+} multiplet (marked by black dots in Fig. 2a) and the conductance dip at zero bias (V = 0), result from singleion Kondo physics^{7}. Specifically the latter signifies the hybridization between 4f and conduction electrons. The most striking feature, however, is the evolution of the peak at about −6 mV (red arrow in Fig. 2a). This peak initially develops below 30 K, but clearly dominates the spectra only for \(T \lesssim 3.3\,{\mathrm{K}}\).
We now focus on this lowtemperature regime T ≤ 3.3 K (Fig. 2b). These data were obtained on the surface shown in the inset where topography over an area of 20 × 10 nm^{2} is presented. Such a topography not only attests the excellent sample quality but is also indicative of Si termination (see Supplementary Note 1 and Supplementary Figs. 1, 2). This termination is pivotal to our discussion as it implies predominant tunneling into the conduction electron states. A hint toward the origin of the −6 mVpeak comes from renormalized band structure calculations^{33}: a partially developed hybridization gap is seen in the quasiparticle DOS at slightly smaller energy. Here, as a result of the renormalization the 4f band is shifted close to the Fermi level. Since tunneling spectroscopy on Siterminated surfaces primarily probes conduction electrons and the total number of electrons must remain constant, the hybridization gap in the 4fband is seen as a peak in our tunneling spectroscopy. On the other hand, a multilevel, finiteU noncrossing approximation (NCA) described our temperaturedependent tunneling spectra away from the energy range of this peak reasonably well^{7} but presented no indication for the existence of a peak at −6 mV. Since NCA does not include intersite Kondo correlations it is very reasonable to assume that this peak results from a strong development of lattice coherence, i.e. the lattice Kondo effect, and will be referred to as the Kondo lattice peak. The bulk nature of the −6 mV peak is supported by comparison to bulk transport measurements, as discussed below.
An analysis of the Kondo lattice peak is impeded by the strongly temperaturedependent zerobias dip close by (see also Fig. 3d, Supplementary Notes 2, 3 and Supplementary Figs. 3, 4). Data \(g( V,T \,\gtrsim \, 30\,{\mathrm{K}} )\) for −15 mV ≤ V ≤−3 mV can be well approximated by a parabola and hence, we assume a parabola to describe the background below the Kondo lattice peak at low temperature, see the example of T = 0.3 K in Fig. 3a. There are finite energy ranges on both sides of the peak feature allowing to fit a parabola, cf. arrows in Fig. 3a. After background subtraction, each peak can be well described by a Gaussian (lines in Fig. 3b) from which its height and width (full width at half maximum, FWHM) is extracted. Note that the peak position in energy is independent of temperature (Fig. 3b). Clearly both, the peak height and FWHM, exhibit a significant change across T_{P} ≈ 3.3 K, Fig. 3c. In contrast, the dip in zerobias conductance, the hallmark of the singleion Kondo effect, smoothly continues to deepen (Fig. 3d, for data on linear Tscale see Supplementary Fig. 4). Here, the depth of the zerobias dip is defined as \(1  [g(V = 0,T)/g(V =  80\,{\mathrm{mV}},T)]\)^{7}. This depth decreases logarithmically for 10 K < T ≤ 120 K, i.e. around T_{K}, as predicted by dynamical mean field theory^{34}.
Comparison to magnetotransport and thermopower measurements
While this temperature evolution of the singleparticle spectrum is surprising, it connects well with the features that appear in bulk transport measurements^{14,15,16,17,35,36}. Importantly, Fig. 4 shows that the thermopower divided by temperature, −S/T, has a qualitatively similar temperature dependence as the height of the STS Kondo lattice peak. Both display a plateau below about 7 K, and a subsequent strong increase upon lowering the temperature below T_{P} ≈ 3.3 K. Here, T_{P} is defined as the temperature at which the −6 meVpeak strongly develops. In the zerotemperature limit, a Fermi liquid is characterized by a constant value S/T. For a Kondo lattice system, this is expected to be seen at very low temperatures, i.e., once the renormalized band structure is almost fully developed^{37}. In fact, for YbRh_{2}Si_{2} heavy Fermiliquid behavior was observed beyond the QCP: At fields μ_{0}H = 1 T, the coefficient −S/T reaches ≈ 7 μV/K^{2} for temperatures up to ~0.5 K^{35}, indicative of a very large effective charge carrier mass. The plateau in S/T seen in Fig. 4 occurs at a value almost an order of magnitude smaller and extends to a correspondingly higher temperature (see also Supplementary Note 5). This indicates some medium heavy Fermi liquid, i.e. prevailing Kondolattice correlations. Moreover, the nearly logarithmic increase in S/T below T_{P} resembles that of the Sommerfeld coefficient γ of the electronic specific heat^{14} and is a clear signature of nonFermi liquid behavior^{35}. Therefore, the comparison of our STS results with those of S/T naturally leads us to propose that the incipient saturation of the Kondo lattice peak height below about 7 K (Fig. 4) signifies some prevailing Kondo–lattice correlations and, importantly, the growth of this peak below T_{P}, as well as the concomitant drop of peak width (Fig. 3c) capture the quantum critical behavior. This leads to the insight that quantum criticality arises not before there is sufficient buildup of lattice Kondo correlations (see Supplementary Note 4 and Supplementary Fig. 5), or conversion of the local 4f electron spins into extended quasiparticlelike, but still incoherent excitations.
To illustrate this point further, the Hall mobility μ_{H} = R_{H}/ρ_{xx} as a function of temperature is also plotted in Fig. 4, right inset (R_{H} itself is compared to S/T in Supplementary Fig. 6). In the regime where the anomalous Hall effect dominates, this quantity has been considered as capturing the buildup of the onsite Kondo resonance^{38}. It is striking that the Hall mobility also shows a strong increase upon lowering the temperature. Yet, the Hall mobility does not show any plateau near 3 K, and neither does the resistivity nor the Sommerfeld coefficient as a function of temperature^{14}. This implies that T_{P} ≈ 3.3 K is not an ordinary Fermi liquid scale. The connection between the growth of the Hall mobility with quantum criticality becomes evident when we analyze its inverse 1/μ_{H} = ρ_{xx}/R_{H}, which is equivalent to the cotangent of the Hall angle, cot θ_{H}, as a function of temperature. In YbRh_{2}Si_{2}, a powerlaw behavior of 1/μ_{H}, more specifically 1/μ_{H} ~ T^{2}, is observed for 0.5 K \(\lesssim T \lesssim\) 5 K (see Supplementary Fig. 7). Such a behavior, as well as the Tlinear electrical resistivity seen in relevant parts of the phase diagram of YbRh_{2}Si_{2}^{14}, has also been observed, e.g., in the cuprate highT_{c} superconductors^{39}.
Evolution of tunneling spectra in magnetic fields
To search for more direct STS evidence for quantum criticality in the H–T phase diagram of YbRh_{2}Si_{2}, the system was tuned by a magnetic field at T = 0.3 K ≈ 0.1T_{P}, i.e. where coherent lattice effects are clearly dominating. Some g(V, H, T = 0.3 K)curves are presented in Fig. 5a. No major change in the overall shape of the spectra with magnetic field is observed. The Kondo lattice peak can again be described by a Gaussian after parabolic background subtraction (Fig. 5b). Within the energy resolution of our STM the peak’s position in energy is independent on H. The resulting FWHM of the peak in dependence on H is presented in Fig. 5c. We note that the FWHM at low T and fixed H varies very little between different spectra, and even different samples, i.e. <4% (see also Fig. 3c where several data points of the FWHM fall on top of each other). This is taken as the error of FWHM, and determines the size of the error bars in Fig. 5c. Moreover, a comparison between the data and the Gaussian fit in Fig. 5b reveals an only slightly enhanced noise of g(V, H, T = 0.3 K) at elevated fields compared to zero field. Consequently, the trend displayed in Fig. 5c appears genuine.
At a field of μ_{0}H = 1 T, the Kondo lattice peak FWHM exhibits a minimum, with a reduction of about 15% of its highfield value. This field is approximately of the value μ_{0}H^{*} ≈ 1.3 T at which the Hall crossover takes place at T = 0.3 K for Hc (red cross in Fig. 5c, for the field direction see Supplementary Note 6). The range in magnetic field over which the Hall crossover is observed^{16} is indicated by a red arrow in Fig. 5c. This implies that changes in g(V, H, T = 0.3 K) are to be expected within a similar field range, as indeed suggested by the drop in peak width vs. H at T = 0.3 K (see also Supplementary Note 7 and Supplementary Fig. 8). Note that at this low temperature Kondo lattice effects are dominating. In this regime, the observed drop of peak width at μ_{0}H = 1 T indicates a reduced quasiparticle weight and follows the expected behavior for a critical slowing down concluded from isothermal magnetotransport (Hall coefficient, R_{H}, and magnetoresistance, ρ_{xx}) measurements^{15,16}, revealing thermally broadened jumps at H^{*}(T). One may therefore expect that the drop in peak width may further increase and sharpen upon cooling, (cf. Fig. 1). In this view, all our findings reflect the finite temperature remnant of a fieldinduced QCP at T = 0. Data from specificheat measurements on YbRh_{2}Si_{2} in magnetic field^{40} confirm this assignment (cf. Supplementary Fig. 8). They yield a relative change of the Sommerfeld coefficient between critical (H^{*}) and elevated fields of order 30% at T = 0.3 K, if scaled for the relevant field orientation. We believe that the larger change in Sommerfeld coefficient compared to the drop in FWHM of the STS Kondo lattice peak (Fig. 5c, about 15% compared to the value at 9 T at which YbRh_{2}Si_{2} is almost in the Fermi liquid regime^{41}) is related to the fact that heat capacity integrates over the whole Brillouin zone while STS is a more directional measurement. For a surface along the a–b plane (Fig. 2), tunneling along the cdirection is most relevant, yet hybridization of the Yb CEF ground state orbitals is anisotropic^{33}, mostly with the Rh \(4d_{x^2  y^2}\).
Remarkably, the FWHM at zero field falls in line with its trend at high fields μ_{0}H ≥ 3.5 T, i.e. there is no significant difference at T = 0.3 K at both sides of the QCP. While the presented STS data on its own do not allow to distinguish between quantum critical scenarios, they are in good agreement with isothermal magnetotransport data. Even at a temperature as low as ~0.5 K, the Hall crossover is expected to reach all the way to H = 0^{13}. In analogy, the peak width in STS at H = 0 should be close to the one extrapolated from higher fields, where a large Fermi surface constitutes the heavy Fermi liquid. Crossing the T^{*}line at temperatures as high as about half a K, there is still a dominating contribution of the large Fermi surface to the quantumcritical fluctuations even at zero field^{42}. Upon cooling, this contribution of the large Fermi surface at H = 0 is expected to decrease^{13}. To establish this trend further, lower temperatures for our STS measurements are clearly called for. We note that Lifshitz transitions and Zeeman splitting can be ruled out as origins for the drop of the peak’s FWHM (see Supplementary Note 5).
Discussion
Our STS studies here have revealed two important insights. One is that the development of the dynamical lattice Kondo correlations in a stoichiometric material such as YbRh_{2}Si_{2}, while setting in at T_{coh} ≈ T_{K}, extends to considerably lower temperatures and dominate the material’s properties only at much lower temperatures (see Supplementary Note 4). In the case of YbRh_{2}Si_{2}, the STS Kondo lattice peak height and thermopower coefficient do not indicate dominant lattice Kondo correlations before the temperature has reached T_{P} ~ 0.1·T_{coh}. Moreover, the conductance minimum at zero bias, which has been shown to capture primarily the onsite Kondo (i.e. hybridization) effect at temperatures \(T \gtrsim 5\,{\mathrm{K}}\)^{7}, also continues to deepen down to the lowest measured temperature as shown in Fig. 3d. Conversely, the strengthening of the lattice Kondo coherence only at much below T_{K} implies that the onsite Kondo effect dominates many thermodynamic and transport properties at around and below T_{coh} in YbRh_{2}Si_{2}, and gives way to the lattice Kondo correlations only slowly upon reducing the temperature. Such a persistence of this distinct signature of the singleion Kondo effect down to temperatures substantially below T_{coh} is consistent with observations based on different transport^{37,38} and thermodynamic^{8,43} properties of several other heavyfermion metals. On the one hand, this provides a natural explanation to the applicability of singleionbased descriptions to temperatures well below T_{K} even though they neglect lattice Kondo coherence effects^{7,37,38}. On the other hand, this finding supports nicely the theoretical concept of two temperature scales, i.e. a singleion and a lattice Kondo scale^{29,30}, including the predicted order of magnitude difference^{30}.
The second lesson concerns the link between the development of the dynamical lattice Kondo correlations and quantum criticality. As a function of temperature, our measurements of the height and width of the Kondo lattice peak strongly suggest that, in order for the quantum criticality to set in, the lattice Kondo correlations first have to develop sufficiently upon lowering the temperature through, and well below, T_{K} ≈ T_{coh} ≅ 30 K. More specifically, as the temperature is lowered through T_{coh}, both the Kondo lattice peak height and the thermopower coefficient first reach a plateau below about 7 K signifying welldeveloped lattice Kondo correlations. It is against this backdrop that the Kondo lattice peak height and S/T markedly increase below T_{P} ≈ 3.3 K. This manifests quantum criticality at the level of the singleparticle spectrum, which goes considerably beyond the quantum critical behavior seen in the divergent Sommerfeld coefficient of the electronic specific heat and the linearinT electrical resistivity^{14}. This signature of the quantum criticality at the singleparticle level is complemented by the isothermal behavior of the Kondo lattice peak with respect to the control parameter, the magnetic field, at the lowest measured temperature, T ≈ 0.3 K. The FWMH of this peak displays a minimum at a similar field value at which isothermal transport and thermodynamic measurements show a Fermi surface crossover^{15,16,17} indicating its relation to quantum criticality.
To put these findings into perspective, our comparative studies indicate an appealingly natural scenario: the development of the lattice Kondo correlations is the prerequisite for quantum criticality. Only if the Kondo lattice is sufficiently established quantum critical fluctuations can evolve. As such, the insights gained in our study will likely be relevant to the nonFermi liquid phenomena in a broad range of other strongly correlated metals, such as the highT_{c} cuprates and the organic chargetransfer salts, which are typically in proximity to Mott insulating states and in which quantum criticality is often observed^{44,45,46}.
Methods
Sample characterization
Highquality single crystals of YbRh_{2}Si_{2} were grown by an indiumflux method; they grow as thin platelets with a height of 0.2–0.4 mm along the crystallographic cdirection (see also Supplementary Note 6). Crystalline quality and orientation of the single crystals were confirmed by xray and Laue investigations, respectively. The residual resistivity ρ_{0} of the six samples investigated here ranged between 0.5 and 0.9 μΩ cm with no apparent differences in their spectroscopic results. The samples were cleaved in situ perpendicular to the crystallographic c direction at temperatures ~20 K. Subsequent to cleaving, the samples were constantly kept under ultrahigh vacuum (UHV) conditions and did not exhibit any sign of surface degradation for at least several months, as indicated by STM reinvestigation.
Scanning tunneling microscopy and spectroscopy
STM and STS was conducted (using a cryogenic STM made by Omicron Nanotechnology) at temperatures between 0.3 and 6 K, in magnetic fields μ_{0}H ≤ 12 T (applied parallel to the crystallographic c direction) and under UHV conditions (p < 2·10^{−9} Pa). Spectroscopic measurements were conducted using lockin technique with V_{rms} = 0.2 mV. For the tunneling spectra shown, g(V, T)data were averaged over areas of 1 × 1 nm^{2} on grids of 24 × 24. In zero magnetic field, the averaging area was repeatedly varied between zero (i.e. spectroscopy repeated at a given point) and 5 × 5 nm^{2} to ensure local homogeneity of the g(V,T)data. For the temperature range 4.6 K ≤ T ≤ 120 K a second UHV STM (LTSTM) was utilized (p ≤ 3·10^{−9} Pa).
Thermopower measurements
The thermopower S was measured by applying a temperature gradient to a rodshaped sample of dimensions 4 × 0.5 × 0.1 mm^{3} out of the same batch as the samples used in STM/S measurements. For low temperatures 0.03 K \(\lesssim T \lesssim\) 6 K, a homebuilt, dilution refrigeratorbased setup was used, while measurements between 2 and 360 K were conducted in a PPMS (Quantum Design Inc.). The overlap of the two temperature ranges between 2 and 6 K serves as consistency check. Thermopower data in the hightemperature range compare nicely to those obtained earlier^{47}. Hall effect measurements (see ref.^{48} for details) were conducted on the same sample as the thermopower measurements.
Data availability
The data that support the findings of this study are available from the corresponding author upon request.
References
Grewe, N. & Steglich, F. in Handbook on the Physics and Chemistry of Rare Earths Vol. 14 (eds. Gschneidner, K. A. Jr. & Eyring, L.) 343–474 (Elsevier, Amsterdam, 1991).
Wirth, S. & Steglich, F. Exploring heavy fermions from macroscopic to microscopic length scales. Nat. Rev. Mater. 1, 16051 (2016).
Doniach, S. Kondo lattice and weak antiferromagnetism. Phys. B 91, 231–234 (1977).
Sachdev, S. Quantum Phase Transitions (Cambridge University Press, Cambridge, 2011).
Coleman, P. & Schofield, A. J. Quantum criticality. Nature 433, 226–229 (2005).
von Löhneysen, H., Rosch, A., Vojta, M. & Wölfle, P. Fermiliquid instabilities at magnetic quantum phase transitions. Rev. Mod. Phys. 79, 1015–1075 (2007).
Ernst, S. et al. Emerging local Kondo screening and spatial coherence in the heavyfermion metal YbRh_{2}Si_{2}. Nature 474, 362–366 (2011).
Pikul, A. et al. Singleion Kondo scaling of the coherent Fermi liquid regime in Ce_{1−x}La_{x}Ni_{2}Ge_{2}. Phys. Rev. Lett. 108, 066405 (2012).
Yang, Y., Fisk, Z., Lee, H.O., Thompson, J. D. & Pines, D. Scaling the Kondo lattice. Nature 454, 611–613 (2008).
Yang, Y. Twofluid model for heavy electron physics. Rep. Prog. Phys. 79, 074501 (2016).
Jang, S. et al. Evolution of the Kondo lattice electronic structure above the transport coherence temperature. Preprint at http://arxiv/abs/1704.08247 (2017).
Chen, Q. Y. et al. Band dependent interlayer felectron hybridization in CeRhIn_{5}. Phys. Rev. Lett. 120, 066403 (2018).
Paschen, S. et al. Kondo destruction in heavy fermion quantum criticality and the photoemission spectrum of YbRh_{2}Si_{2}. J. Magn. Magn. Mater. 400, 17–22 (2016).
Custers, J. et al. The breakup of heavy electrons at a quantum critical point. Nature 424, 524–527 (2003).
Paschen, S. et al. Halleffect evolution across a heavyfermion quantum critical point. Nature 432, 881–885 (2004).
Friedemann, S. et al. Fermisurface collapse and dynamical scaling near a quantumcritical point. Proc. Natl Acad. Sci. USA 107, 14547–14551 (2010).
Gegenwart, P. et al. Multiple energy scales at a quantum critical point. Science 315, 969–971 (2007).
Si, Q. et al. Kondo destruction and quantum criticality in Kondo lattice systems. J. Phys. Soc. Jpn. 83, 061005 (2014).
Küchler, R. et al. Divergence of the Grüneisen ratio at quantum critical points in heavy Fermion metals. Phys. Rev. Lett. 91, 066405 (2003).
Tokiwa, Y., Radu, T., Geibel, C., Steglich, F. & Gegenwart, P. Divergence of the magnetic Grüneisen ratio at the fieldinduced quantum critical point in YbRh_{2}Si_{2}. Phys. Rev. Lett. 102, 066401 (2009).
Gegenwart, P. et al. Magneticfield induced quantum critical point in YbRh_{2}Si_{2}. Phys. Rev. Lett. 89, 056402 (2002).
Abrahams, E. & Wölfle, P. Critical quasiparticle theory applied to heavy fermion metals near an antiferromagnetic quantum phase transition. Proc. Natl Acad. Sci. USA 109, 3238–3242 (2012).
Wölfle, P. & Abrahams, E. Spinflip scattering of critical quasiparticles and the phase diagram of YbRh_{2}Si_{2}. Phys. Rev. B 92, 155111 (2015).
Miyake, K. & Watanabe, S. Unconventional quantum criticality due to critical valence transition. J. Phys. Soc. Jpn. 83, 061006 (2014).
Fischer, Ø., Kugler, M., MaggioAprile, I., Berthod, C. & Renner, C. Scanning tunneling spectroscopy of hightemperature superconductors. Rev. Mod. Phys. 79, 353–419 (2007).
Schmidt, A. R. et al. Imaging the Fano lattice to ‘hidden order’ transition in URu_{2}Si_{2}. Nature 465, 570–576 (2010).
Aynajian, P. et al. Visualizing heavy fermions emerging in a quantum critical Kondo lattice. Nature 486, 201–206 (2012).
Köhler, U., Oeschler, N., Steglich, F., Maquilon, S. & Fisk, Z. Energy scales of Lu_{1−x}Yb_{x}Rh_{2}Si_{2} by means of thermopower investigations. Phys. Rev. B 77, 104412 (2008).
Burdin, S., Georges, A. & Grempel, D. R. Coherence scale of the Kondo lattice. Phys. Rev. Lett. 85, 1048–1051 (2000).
Costi, T. A. & Manini, N. Lowenergy scales and temperaturedependent photoemission of heavy fermions. J. Low Temp. Phys. 126, 835–866 (2002).
Mo, S.K. et al. Emerging coherence with unified energy, temperature, and lifetime scale in heavy fermion YbRh_{2}Si_{2}. Phys. Rev. B 85, 241103(R) (2012).
Kummer, K. et al. Temperatureindependent Fermi surface in the Kondo lattice YbRh_{2}Si_{2}. Phys. Rev. X 5, 011028 (2015).
Zwicknagl, G. Fieldinduced suppression of the heavyfermion state in YbRh_{2}Si_{2}. J. Phys. Condens. Matter 23, 094215 (2011).
Costi, T. A. Kondo effect in a magnetic field and the magnetoresistivity of Kondo alloys. Phys. Rev. Lett. 85, 1504–1507 (2000).
Hartmann, S. et al. Thermopower evidence for an abrupt Fermi surface change at the quantum critical point of YbRh_{2}Si_{2}. Phys. Rev. Lett. 104, 096401 (2010).
Kimura, S. et al. Optical observation of nonFermiliquid behavior in the heavy fermion state of YbRh_{2}Si_{2}. Phys. Rev. B 74, 132408 (2006).
Sun, P. & Steglich, F. Nernst effect: evidence of local Kondo scattering in heavy fermions. Phys. Rev. Lett. 110, 216408 (2013).
Coleman, P., Anderson, P. W. & Ramakrishnan, T. V. Theory for the anomalous Hall constant of mixedvalence systems. Phys. Rev. Lett. 55, 414–417 (1985).
Chien, T. R., Wang, Z. Z. & Ong, N. P. Effect of Zn impurities on the normalstate Hall angle in singlecrystal YBa_{2}Cu_{3−x}Zn_{x}O_{7−δ}. Phys. Rev. Lett. 67, 2088–2091 (1991).
Oeschler, N. et al. Lowtemperature specific heat of YbRh_{2}Si_{2}. Physica B 403, 1254–1256 (2008).
Custers, J. QuantumCritical Behavior in the HeavyFermion Compounds YbRh _{2} Si _{2} and CeIn _{3−x} Sn _{x}. PhD Thesis, Technical University Dresden (2004).
Senthil, T. Critical Fermi surfaces and nonFermi liquid metals. Phys. Rev. B 78, 035103 (2008).
Pietri, R., Rotundu, C. R., Andraka, B., Daniels, B. C. & Ingersent, K. Absence of Kondo lattice coherence effects in Ce_{0.6}La_{0.4}Pb_{3}: a magneticfield study. J. Appl. Phys. 97, 10A510 (2005).
Lee, P. A., Nagaosa, N. & Wen, X.G. Doping a Mott insulator: physics of hightemperature superconductivity. Rev. Mod. Phys. 78, 17–85 (2006).
Ramshaw, B. J. et al. Quasiparticle mass enhancement approaching optimal doping in a highT _{c} superconductor. Science 348, 317–320 (2015).
Oike, H., Miyagawa, K., Taniguchi, H. & Kanoda, K. Pressureinduced Mott transition in an organic superconductor with a finite doping level. Phys. Rev. Lett. 114, 067002 (2015).
Hartmann, S. et al. Thermal transport properties of the heavyfermion compound YbRh_{2}(Si_{1−x}Ge_{x})_{2}. Physica B 378, 70–71 (2006).
Friedemann, S. et al. The crossedfield and singlefield Hall effect in LuRh_{2}Si_{2}. Phys. Status Solidi B 247, 723–726 (2010).
Acknowledgements
We sincerely thank U. Stockert for help with the experiments and discussions, as well as J.C. Séamus Davis for discussions. Work was partly supported by the German Research Foundation through DFG Research Unit 960 and through DFG grant KR3831/41. Work at Rice University has been supported by the NSF Grant DMR1611392, the ARO grant no. W911NF1410525, and the Robert A. Welch Foundation Grant no. C1411. Q.S. graciously acknowledges the support of the Alexander von Humboldt Foundation, the hospitality of the Karlsruhe Institute of Technology, and a QuantEmX grant from ICAM and the Gordon and Betty Moore Foundation through Grant no. GBMF5305. S.K. acknowledges support by the National Key R&D Program of the MOST of China (Nos. 2016YFA0300202 and 2017YFA0303100) and the National Science Foundation of China (Nos. 11474250 and 11774307).
Author information
Authors and Affiliations
Contributions
S.W. and F.S. designed the research. S.S., L.J. and S.W. conducted the STM experiments, S.H. the thermopower measurements and S.F. the Hall measurements. C.K. and C.G. provided the samples. S.K. and Q.S. provided theoretical insight. All authors contributed to the discussions and the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Seiro, S., Jiao, L., Kirchner, S. et al. Evolution of the Kondo lattice and nonFermi liquid excitations in a heavyfermion metal. Nat Commun 9, 3324 (2018). https://doi.org/10.1038/s41467018058015
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41467018058015
This article is cited by

Inducing and tuning Kondo screening in a narrowelectronicband system
Nature Communications (2022)

Superconductivity in an extreme strange metal
Nature Communications (2021)

Artificial heavy fermions in a van der Waals heterostructure
Nature (2021)

Quantum phases driven by strong correlations
Nature Reviews Physics (2020)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.